Electrical Conducting and Magnetic Properties of (Ethylenedithiotetrathiafulvalenothioquinone-1,3-diselenolemethide)2 .FeBr4(GaBr4) Crystals with Two Different Interlayer Arrangements of Donor Molecules
Takuya Matsumoto; Yohsuke Kamada; Toyonari Sugimoto; Toshiji Tada; Satoru Noguchi; Hiroyuki Nakazumi; Motoo Shiro; Harukazu Yoshino; Keizo Murata; Inorganic Chemistry 42 (2003) 5192–5201; doi:10.1021/ic030083v

data_4314017
_publ_contact_author_email       toyonari@iwate.riast.osakafu-u.ac.jp
_publ_contact_author_fax         0722-52-4175
_publ_contact_author_name        'T, Matsumoto'
_publ_contact_author_phone       0722-52-4175
_publ_section_title
;
 Electrical Conducting and Magnetic Properties of
 (Ethylenedithiotetrathiafulvalenothioquinone-1,3-diselenolemethide)2
 .FeBr4(GaBr4) Crystals with Two Different Interlayer Arrangements of
 Donor Molecules
;
_journal_name_full               'Inorganic Chemistry'
_journal_page_first              5192
_journal_page_last               5201
_journal_paper_doi               10.1021/ic030083v
_journal_volume                  42
_journal_year                    2003
_chemical_formula_moiety         '2(C11 H6 S7 Se2 0.5+), Br4 Ga1 1-'
_chemical_formula_sum            'C22 H12 Br4 Ga S14 Se4'
_chemical_formula_weight         1430.35
_space_group_IT_number           14
_symmetry_cell_setting           monoclinic
_symmetry_Int_Tables_number      14
_symmetry_space_group_name_Hall  '-P 2ybc'
_symmetry_space_group_name_H-M   'P 1 21/c 1'
_cell_angle_alpha                90
_cell_angle_beta                 103.37(3)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   7.512(3)
_cell_length_b                   37.59(1)
_cell_length_c                   14.073(5)
_cell_measurement_reflns_used    26338
_cell_measurement_temperature    296.2
_cell_measurement_theta_max      30.1
_cell_measurement_theta_min      3.0
_cell_volume                     3866(2)
_computing_cell_refinement       PROCESS-AUTO
_computing_data_collection       PROCESS-AUTO
_computing_data_reduction        'teXsan Ver. 1.10'
_computing_publication_material  'teXsan Ver. 1.10'
_computing_structure_refinement  'teXsan Ver. 1.10'
_computing_structure_solution    SIR97
_diffrn_detector_area_resol_mean 10
_diffrn_measured_fraction_theta_full 0.9986
_diffrn_measured_fraction_theta_max 0.9986
_diffrn_measurement_device_type  'Rigaku RAXIS-RAPID Imaging Plate'
_diffrn_measurement_method       \w
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.7107
_diffrn_reflns_av_R_equivalents  0.115
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       48
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       17
_diffrn_reflns_limit_l_min       -18
_diffrn_reflns_number            37647
_diffrn_reflns_theta_full        27.49
_diffrn_reflns_theta_max         27.49
_exptl_absorpt_coefficient_mu    9.401
_exptl_absorpt_correction_T_max  0.829
_exptl_absorpt_correction_T_min  0.303
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   '(Higashi, 1995)'
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    2.457
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_size_max          0.300
_exptl_crystal_size_mid          0.100
_exptl_crystal_size_min          0.020
_refine_diff_density_max         3.06
_refine_diff_density_min         -1.92
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.008
_refine_ls_hydrogen_treatment    noref
_refine_ls_number_parameters     406
_refine_ls_number_reflns         8866
_refine_ls_R_factor_gt           0.0622
_refine_ls_shift/su_max          0.0006
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w = 1/[\s^2^(Fo^2^) + (0.03000(Max(Fo^2^,0) + 2Fc^2^)/3)^2^]'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_ref         0.1287
_reflns_number_gt                3802
_reflns_number_total             8866
_reflns_threshold_expression     F^2^>2.0\s(F^2^)
_cod_data_source_file            ic030083v_6.cif
_cod_data_source_block           opu2a
_cod_original_formula_sum        'C22 H12 Br4 Ga S14 Se4 '
_cod_database_code               4314017